Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
∗
†
Abstract
This paper presents a generalization of traditional continuum approaches to liquid crystals and liquid crystal elastomers to allow for dynamically evolving line defect distributions. In analogy with recent mesoscale models of dislocations, we introduce fields that represent defects in orientational and positional order through the incompatibility of the director and deformation ‘gradient’ fields.
These fields have several practical implications: first, they enable a clear separation between energetics and kinetics; second, they bypass the need to explicitly track defect motion; third, they allow easy prescription of complex defect kinetics in contrast to usual regularization approaches; and finally, the conservation form of the dynamics of the defect fields has advantages for numerical schemes.
We present a dynamics of the defect fields, motivating the choice physically and geometrically.
This dynamics is shown to satisfy the constraints, in this case quite restrictive, imposed by materialframe indifference. The phenomenon of permeation appears as a natural consequence of our kinematic approach. We outline the specialization of the theory to specific material classes such as nematics, cholesterics, smectics and liquid crystal elastomers.
Liquid crystals are composed of rodlike molecules. Depending on temperature, chemical composition and other factors, assemblies of the molecules display varying degrees of orientational and positional order. Applied loads such as stress fields cause deformation but also changes in orientation and both these changes cost energy. Hence, the orientation of the molecule is important to elasticity and deformation.
Therefore, coarsegrained continuum theories retain orientation information through the director field that provides a unitvector aligned along the long axis of the molecule. The deformations of liquid crystals can then be described through internal energies that include the director field and its gradient as argument
∗
Email: acharyaamit@cmu.edu
†
Email: kaushik@cmu.edu
1
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
[e.g.,
Ste04 ]. When the liquid crystal molecules are linked to polymer molecule backbones, director
elasticity is strongly coupled to conventional positional elasticity and the internal energy density involves both contributions [e.g.,
WT07 ]. In addition, defects in both orientational and positional order (e.g.
Defectfree liquid crystals have been studied for many decades through continuum approaches, most
notably the EricksenLeslie (EL) [ Eri61 ,
Les68 ] model. The EL model is widely accepted and experi
mentally wellcharacterized through the measurement of the various parameters in the model. However, certain types of observed defects such as disclinations , where the orientation of the director is ambiguous along curves in the body, cannot be predicted by the EL model, in particular disclinations of strength
1
. Such defects, and others such as dislocations and focal conics, have been observed in both static and
2 dynamic situations [e.g.,
This paper generalizes the EL dynamical theory of liquid crystals to allow for solid like behavior as
in the liquid crystal elastomer [ WT07 ] phase and deal with defects in the director
( n ) and position
( x ) configurations, including disclinations and dislocations. The defects are viewed as nonsingular localizations in physically appropriate fields representing densities of lines carrying vectorial attributes.
Being spatial densities, they naturally satisfy balance laws, thus providing a direct geometric route to specify defect dynamics.
The main idea is to allow for smooth incompatibilities in the director and deformation ‘gradient’ fields, henceforth referred to as the corresponding distortion tensors since they are not globally irrotational (curlfree). We do this by introducing defect fields that represent these incompatibilities. This is an expedient device to deal with topological defects without having to deal with discontinuities in the basic fields
( n , x ) whose generalized gradients could be strongly singular. We emphasize that allowing for smooth, incompatible distortion fields is not the same as smoothing the director/position fields in any sense since no continuous global vector field can be defined whose generalized gradient may be equated to the smooth incompatible distortion field. In fact, roughly speaking, if E is a sufficiently smooth director distortion field on the body, it can be written in the form
E = grad n + curl ˆ through a StokesHelmholtz decomposition, where n is a vector field and free) secondorder tensor field.
ˆ is a solenoidal (divergence
ˆ is directly related to the awayfromgradient defect content of E defined by
β := curl E = − div grad ˆ .
Thus, our approach naturally produces a tensor orientational order parameter
ˆ that arises only in the presence of director field defects. It is not necessarily symmetric as the standard Q tensor of Landau
DeGennes theory and neither does it have physical association to headtotail symmetry.
As our model works with a director field and an incompatible director distortion field, it does not share the elegance of the headtotail symmetry in the Q tensor formalism. However, the very generality of the Q tensor construct in representing defects through its spectral decomposition makes it difficult to
Q tensor based on kinetic theorylike ideas [e.g.,
YFMW09 ], originally developed for the
swered questions of constitutive closure – precisely, the closure law for the fourth moment of the angular orientation distribution function – we see pursuing physically faithful continuum mechanics models of
2
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal the same mesoscale phenomena that allow precisely defined constitutive input from either experiment or theory as a useful research path.
Our point of view hence relies on the definition of geometrically precise order parameters for posing conservation laws with physically unambiguous ingredients amenable to constitutive input from finer length scales. Thus, the β
defect tensor has the natural interpretation of a ‘vectorvalued’ twoform 1
that naturally lends itself to integration over surface patches allowing recourse to the standard kinematic tautology “rate of change = flux in + source,” to specify dynamics through balance laws. These are made materialspecific by the addition of constitutive equations. Admittedly, a great deal rests on accurate modeling of the flux and source terms, but the basic format of such equations of evolution, for a rigorously defined and physically natural spatial density, is a useful kinematic fact. In addition, merely from the kinematical fact that these twoforms can be physically interpreted as a field density of lines, a natural consequence is that their flux admits a velocity that moves the lines, thus allowing defect kinetics to
be specified independently from model energetics. By recourse to ColemanNollGurtin [ CN63 , CG67 ]
thermodynamic reasoning in spirit, we set up a multiscale, dynamical, PDE model with favorable dissipative properties while allowing for energetic and kinetic input from molecular scales. Also, tying the identity of defects to values of a field has the practical advantage that individual defects do not need to be tracked as discontinuities or singularities in numerical computations.
The model also allows for accommodating the standard OseenZocherFrank (OZF) [ Ose33 ,
grad n =: G by E in the that energy density. Since defects can be represented here as nonsingular localizations of the director incompatibility field, the OZF energy of the body containing defects can be bounded in the model. As in the crystal elasticity case [e.g.,
is possible that nonconvexity in the OZF energy is required to obtain localized defect cores. This may be justified for large director distortions (as no elasticity can persist indefinitely), and a physical regularization for avoiding singularities, attributed to extra core energy, is also accommodated. We find it particularly satisfying that our model incorporates defects within OZF orientational elasticity without any additional elasticity related to the ‘degree of orientation’ variable, a feature in contrast with Ericksen
[ Eri91 ] and discussed at some length therein.
The nematic, cholesteric, and smectic (A and C) liquid crystal phases, the nematic and smectic liquid crystal elastomer phases can all be modeled in our formulation by appropriately restricting the kinematics and using standard generalizations of the OZF energy. In the smectic phase, a permeation velocity field appears on purely kinematic grounds. We note that its spatial gradient is conceptually similar to
compatible plastic strain rate (e.g. lattice invariant shears) in crystal plasticity [ DP91 ,
A special case of our model is a dissipative, dynamic, nonlinear theory of elasticity with dislocations
emerges for treatment of director incompatibility and dislocation defect evolution. It is characterized in the most simple of circumstances by a scalar equation of the form
φ t
=
 φ x

[ φ xx
+ τ ( φ )]
B where 0 < 1 , 0 < B are material parameters and τ
is a nonconvex function [ Ach10 , AMZ10 ].
We do not provide a comprehensive review of the vast literature relevant to a dynamic model of liquid crystalline materials. Our understanding of liquid crystal materials has greatly benefited from the books
], Stewart [ Ste04 ], and Warner and Terentjev [ WT07 ]; the papers of
1
That is, a rigorously defined areal density on a manifold in Euclidean space.
3
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
], and Stephen and Straley [ SS74 ]. Beyond
practical computation, it is clear that the nonlinear PDE structure that emerges here will benefit from rigorous mathematical analysis to understand the finer points of defect dynamics and microstructure [e.g.,
GHL + 10 ], and continues to be studied within the
Q tensor formalism, e.g.
line defects. There is an emerging body of work due to Fried and coworkers [e.g.,
configurationalforce approach to defect dynamics in liquid crystalline materials, and understanding the connections with our approach would be useful.
The paper is organized as follows:
• Section
provides notation and some definitions
• Section
outlines the balance laws
• Section
deals with the geometry and evolution of director line defects
• Section
deals with the geometry and evolution of dislocations
• Section
summarizes the field equations including those of the defects
• Sections
and
examine the restrictions imposed by frameindifference and thermodynamics
• Section
outlines the constitutive choices to model various classes of liquid crystal materials
• Section
concludes with a discussion
• Appendix
provides practical strategies to connect with observed fields
• Appendix
discusses disclinations and some classical static defect solutions from the perspective of our model
A superposed dot on a symbol represents a material time derivative. The statement a := b indicates that a is defined to be equal to b . The summation convention is implied unless otherwise mentioned. We denote by Ab the action of the secondorder (thirdorder, fourthorder) tensor A on the vector (secondorder tensor, secondorder tensor) b , producing a vector (vector, secondorder tensor). A · represents the inner product of two vectors, a : represents the trace inner product of two secondorder tensors (in rectangular
Cartesian components, A : B = A ij
B ij
) and matrices and the contraction of the last two indices of a thirdorder tensor with a second order tensor. The symbol AB represents tensor multiplication of the secondorder tensors A and B . The notation ( · ) sym and ( · ) skw represent the symmetric and skew symmetric parts, respectively, of the second order tensor ( · ) . The symbol div represents the divergence, grad the gradient, and div grad the Laplacian. The curl operation and the cross product of a secondorder tensor
4
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal and a vector are defined in analogy with the vectorial case and the divergence of a secondorder tensor: for a secondorder tensor A , a vector v , and a spatially constant vector field c ,
( A × v )
T c = A
T c × v ∀ c
(div A ) · c = div A
T c ∀ c
(curl A )
T
· c = curl A
T c ∀ c .
In rectangular Cartesian components,
( A × v ) im
= e mjk
A ij v k
(div A )
(curl A ) im i
= A ij,j
= e mjk
A ik,j
.
where e mjk is a component of the thirdorder alternating tensor X . Also, the vector XAB is defined as
( XAB ) i
= e ijk
A jr
B rk
.
The spatial derivative for the component representation is with respect to rectangular Cartesian coordinates on the current configuration of the body. For manipulations with components, we shall always use such rectangular Cartesian coordinates. Positions of particles are measured from the origin of this arbitrarily fixed Cartesian coordinate system. We use the identity curl curl( · ) = grad div( · ) − div grad( · ) , often for an argument for which div( · ) = 0 .
The following list describes some of the mathematical symbols we use in this paper.
n : director x : current position
E : director distortion tensor
F
W e
: elastic distortion tensor
= ( F e
)
− 1
: inverse of elastic distortion tensor
β : director incompatibility tensor
α : dislocation density tensor v : material velocity
ω : director angular velocity; ˙ = ω × n
L : velocity gradient
D = L sym
: rate of deformation tensor
Ω = L skw
: spin tensor
G = grad n : director gradient tensor
M = grad ω : director angular velocity gradient
T : Cauchy stress tensor
Λ : couple stress tensor
Γ : skewsymmetric tensor corresponding to ω ; Γ := Xω
R : rotation tensor defined from Γ ; RR
T
= − Γ p : permeation velocity
K : external body moment per unit mass b : external body force per unit mass
ρ : mass density
ψ : free energy per unit mass
5
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
β
V : director incompatibility velocity
α V : dislocation velocity
In contrast to standard EL theory, we relax the requirement that the director distortion be the gradient of a vector field. Due to incompatibility, the constraints on G arising from the fixed length of the director
CF06 ] cannot be translated to a constraint on
E
. Thus, we follow in spirit Leslie [ Les68 ] and,
more generally, liquid crystal theories with variable degree of orientation to adopt a compatible director field that is not necessarily of fixed length, but allow only small deviations from the fixed length by appropriate constitutive energetic penalty.
The symbol
(
˚
) = div v ( · ) + (
˙
· ) − ( · ) L
T
(2.1) for a secondorder tensor argument ( · ) is defined as the “backleg, contravariant, convected derivative with respect to the timedependent tensor function J F ” of that tensor, where F is the deformation gradient with respect to an arbitrarily chosen fixed reference configuration and J = det F . This convected derivative arises most naturally in connection with twopoint tensor fields whose domain is a tangent
Finally, we use the notion of a 2 form in a 3 d Euclidean space interchangeably with the vector representation of its adjoint 1
For any fixed set of material particles occupying the volume V ( t ) at time t with boundary ∂V ( t ) having outward unit normal field ν
Z
V ( t )
˙
ρ dv = 0 ,
Z
V ( t )
˙
ρ v dv =
Z
∂V ( t )
T ν da +
Z
V ( t )
ρ b dv,
Z
V ( t )
˙
ρ x × v + n ×
· n dv =
Z
∂V ( t )
( x × T + Λ ) ν da +
Z
V ( t )
ρ ( x × b + K ) dv, represent the statements of balance of mass, linear and angular momentum, respectively. In geometric language appropriate to Euclidean space, one can think of mass as a scalarvalued 3 form (i.e., a ‘true’ differential form that has meaning apart from the Euclidean structure), and linear momentum and angular momentum as vectorvalued 3
forms. Here, we have followed [ ACF99 ] in defining the director contri
forms for these equations are:
ρ ˙ + ρ div v = 0
ρ ˙ = div T + ρ b
ρ n × ¨ = div Λ − X : T + ρ K .
2 While allowing for the relaxation of the unit vector constraint on the director.
(3.1)
6
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
The external power supplied to the body at any given time is expressed as:
P ( t ) =
=
Z
Z
V ( t )
ρ b · v dv +
Z
∂V ( t )
( T ν ) · v da +
Z
∂V ( t )
( Λν ) · ω da +
Z
V ( t )
ρ K · ω dv
Z
( ρ v · ˙ + ρ ˙ · ¨ ) dv + ( T · L + Λ : M + T : Γ ) dv.
V ( t ) V ( t )
On defining the generalized kinetic energy and the free energy of the body as
K =
Z
Z
V ( t )
1
2
( ρ v · v + ρ ˙ · n ) dv,
F = ρψ dv,
V ( t ) respectively, and using Reynold’s transport theorem, we obtain the mechanical dissipation
D := P − K
˙
F =
Z
V ( t )
T : L + Λ : M + T : Γ − ρ ψ
˙ dv.
(3.2)
The first equality above shows the distribution of applied mechanical power into kinetic, stored and dissipated parts. The second equality, as we show subsequently, is used to identify driving forces for dissipative mechanisms.
We define the director incompatibility tensor as the departure of the director distortion from being the director gradient. So, curl E = curl( E − G ) =: β .
(4.1)
Both E and β are tensor fields on the current configuration, i.e., their values at any given point on the current configuration act on vectors from the tangent space at that point and produce vectors on the same tangent space. Therefore, if the current configuration is subjected to a rigid rotation characterized by a tensor Q , then E transforms to the fields QEQ
T on the rotated configuration and similarly for β .
The definition of G as a spatial gradient suggests that it is a vectorvalued 1 form, i.e., an object that can be integrated on curves to produce a vector. In the absence of defects E = G , and hence E belongs to the
same class of geometric objects. By ( 4.1
β is an areal density of defect lines, including disclinations, that represents director nonintegrability. This is best appreciated at a spatial point where β can be written as a tensor product of two vectors, so that the defect density may be visualized as a line carrying a vectorial attribute (Figure
a is any oriented area patch with unit normal field ν and bounded by the closed curve c , and a has no defect lines intersecting it, then E can be written as a gradient on the patch. On the other hand, for an area patch intersected by the defect line, the integral
Z a
βν da
7
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal quantifies the failure of E to define a singlevalued director field when integrated along the closed curve c . Thus
βν da characterizes the director vector defect content in the oriented infinitesimal area element ν da . Hence, β
is a vectorvalued twoform. An immediate consequence of the definition ( 4.1
β is a solenoidal field and this implies that the defect lines either end at boundaries or are closed loops.
Figure 1: Director incompatibility defect lines.
It is natural to assume that these linelike objects move with a velocity and thus a velocity field β V , relative to the material, can be attributed to the director incompatibility field. The defect density field may also be integrated over an area and an accounting of the defect content of a particular areapatch of material particles over time can be carried out. This is the basis of the conservation laws that provide the dynamics of such fields. In posing this dynamical statement, a central goal is to stay as close as possible
to the EL [ Les92 ] theory. In particular, it is desirable that:
1. the EL dissipation is augmented only by the motion of director incompatibility defects (e.g. disclinations) and dislocations, and the occurrence of permeation,
2. the governing equations and constitutive equations are stated in terms of the current state of the material and information on the current configuration, without reference to prior states except for defining positional elastic response, and
3. the theory is consistent with material frameindifference.
As we demonstrate, a conservation law that is consistent with these three requirements is of the form
Z a ( t )
˙
βν da = −
Z c ( t )
β × β
V d x −
Z a ( t )
(curl ( Γ ( E − G ))) ν da, (4.2) where a ( t ) is the area patch occupied by an arbitrarily fixed set of material particles at time t and c ( t ) is
its closed bounding curve. The corresponding local form of ( 4.2
˚
= − curl β ×
β
V − curl ( Γ ( E − G )) .
8
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
The first term on the right side of ( 4.2
) represents the flux of director incompatibility carried by defect
lines entering the material area patch a . This is best understood by decomposing β and β V on a special orthonormal basis oriented with respect to an infinitesimal segment of the bounding curve c as shown in Figure
2 . Without loss of generality, we also assume that the basis chosen is such that
ν of the infinitesimal area element at the boundary is not parallel to p
1
× p
2 or p
1
× p
3
.
Figure 2: Orientation of local frame for understanding defect flux.
β ×
β
V d x = − dx ( βp i
) ⊗ p i
= − ( βp
1
) dx p
1
×
×
β
V p
1
β
V
1 p
1
+
β
V
2 p
2
+
β
V
3 p
3
− ( βp
2
) dx p
2
× β
V
1 p
1
+
β
V
2 p
2
+
β
V
3 p
3
· p
1
· p
1
− ( βp
3
) dx p
3
× β
V
1 p
1
+
β
V
2 p
2
+
β
V
3 p
3
· p
1
.
Mathematically it is clear that there is no contribution to the flux from the first term on the right side above. Physically, this is because the motion of any defect line along itself clearly produces no flux into the area element. Furthermore the motions along directions p
2 along p
1
, produce no intersection of this line component with the area element. Similar reasoning gives the physical meaning of and p
3
, of the defect line component
− β × β
V d x = − ( βp
2
) dx
β
V
3
+ ( βp
3
) dx
β
V
2
.
Note that the signs are consistent with the chosen orientation of a and c .
The second term on the righthandside of ( 4.2
) represents a geometric source term that enables con
sistency of the conservation law with the first and third requirements above, as we show at the end of
Section
) as an adapted convected derivative as we now show.
Arbitrarily fix an instant of time, say s , in the motion of a body and let F denote the timedependent deformation gradient field corresponding to this motion with respect to the configuration at the time s .
9
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
Denote positions on the configuration at time s as x s and the image of the area patch a ( t ) as a ( s ) . We similarly associate the closed curves c ( t ) and c ( s )
. Then, using the definition ( 4.1
⇒
Z a ( t )
˙
(curl ( E − G )) ν da = −
Z a ( t ) curl β × β
V + Γ ( E − G ) ν da
Z
˙
( E − G ) F d x s
= −
Z c ( s )
β × β
V + Γ ( E − G ) F d x s
Z c ( s )
⇒ curl ( E −
˙
G ) F + β × β
V + Γ ( E − G ) F ν da = 0 a ( s )
⇒ ( E −
˙
G ) F = − β × β
V + Γ ( E − G ) F ,
(4.3) since the conservation law holds for all area patches. Without loss of generality, we have made the assumption that a possibly additive gradient vanishes. Consequently, we have
( E
˙
G ) F + ( E − G ) LF = − β × β
V + Γ ( E − G ) F (4.4) and choosing s = t
( E − G ):= Γ ( E − G ) + ( E
˙
G ) + ( E − G ) L = − β × β
V .
(4.5) where ( E − G )
defines a convected derivative. The reader content with accepting ( 4.2
balance law that satisfies frameindifference and thermodynamics can bypass the following subsection.
We provide there the geometric line of thought for the extremely specific source term and time derivative
For those unfamiliar with the notion of convected (generalized Lie) derivatives, we begin with an example specific to our context that exposes the geometric structure of these time derivatives. Recalling the definition of the orthogonal tensor field R and defining its initial condition as
RR
T
= − Γ ; R ( s ) = I ,
h
R
T
Γ ( E − G ) F + R
T
( E
˙
G ) F + R
T
( E − G ) LF i t = s
= R R
T
˙
( E − G ) F F
− 1 t = s
= ( E − G ) .
Thus, ( E − G ) represents the pushforward of the time derivative of the pullback of E − G by the pointwise timedependent tensor functions R (frontleg) and F
− T
(backleg), evaluated at s = t . Thus it is a mixed, covariant convected derivative which cannot be viewed as a Lie derivative because of the fact that two (moreorless) unrelated timedependent tensor functions are involved in the pullback and pushforward operations, one of which (i.e., R ) may not lend itself to interpretation as a deformation gradient
10
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal of any flow of the basic manifold. To see the resulting convected derivative transparently, consider two sets of timedependent bases c i
( t ) = R ( t ) c i
( s ); e i
( t ) = F ( t ) e i
( s ) , where s is an arbitrarily fixed instant of time. The corresponding dual bases are denoted as ( c i and ( e i : i = 1 , 2 , 3) with c i ( t ) = R ( t ) c i ( s ) and e i ( t ) = F
− T
( t ) e i ( s ) . We write the tensor (
:
E i = 1
−
,
G )
2 , 3) on these mixed bases:
( E − G ) = ( E − G ) ij c i ⊗ e j
; ( E − G ) ij
= c i
· ( E − G ) e j
.
Then,
( E − G )= h
( E −
˙
G ) ij c i
⊗ e j i t = s
= R ( E − G ) ij
R
˙
T c i ⊗ F
T e j F
− 1
.
t = s
It is because of this pullback → time derivative → push forward structure that these derivatives are useful to differentiate a oneparameter family of tensors where the elements of the family do not belong to the same linear space.
We now provide the motivation behind stating the director incompatibility balance in the form ( 4.2
preliminary notion is a desire to write a balance law for densities of lines in the form
Z a ( t )
˙
βν da = −
Z c ( t )
β × V d x .
Localization of the integral balance produces the term
˚ on the left side. However, from its definition,
β ( x , t ) is a tensor that maps a timeevolving tangent space at a point on the current configuration to itself.
Thus, simply adopting a ‘backleg’ convected derivative for β does not make rigorous geometric sense.
Since we are working in Euclidean space, a valid meaning can still be attached to such a derivative, and
in the situation with director incompatibility, such a device does not work; if the free energy density is a function of E , as it is for the materials considered here, the dissipation of the model is not frameindifferent. Summing vectors from tangent spaces of different base points of a manifold, as implied in the writing of an integral, also does not make rigorous geometric sense: however, again, the Euclidean structure allows a meaning to be attached to the integral and, in this case, such an operation does not interfere with frameindifference down the road.
Hence, we define the auxiliary (frontleg) pulledback, twopoint tensor field curl R
T
( E − G ) =: β s
, (4.6) where s
is still the arbitrarily fixed instant of time introduced in connection with ( 4.3
conservation law for β s in the form
Z a ( t )
˙
β s
ν da = −
Z c ( t )
β s × V s d x ∀ t,
3 Balance of linear momentum is an example of a widelyaccepted physical equation that contains a time derivative that is not frameindifferent.
11
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal where V s is the velocity of the β s at time t
. With arguments similar to ( 4.3
R
T
Γ ( E − G ) F + R
T
( E
˙
G ) F + R
T
( E − G ) LF = − β s
× V s for all t with s held fixed. (4.7)
From a mathematical standpoint this is a reasonable expression; however, physically it has the shortcoming that it involves an arbitrary history dependence through the definition of R , F that cannot be relevant in describing the evolution of director distortion or incompatibility. This is not an obstacle, as we evaluate
s = t , since s was fixed arbitrarily. Moreover, the procedure can be repeated for all values of s , fixing s first, performing the time derivative, and then evaluating for s = t , i.e. choosing the current configuration as the reference. Consequently, we arrive at the evolution equation for director distortion
On asking the question of what integral balance law is consistent with ( 4.5
for all instants of time , one
simply reverses the computation of arriving at ( 4.5
specific geometric source term, is the correct statement.
An interesting fact is that from the point of view of using an objective time rate, F
− 1 instead of R
T
could just as well have been used for the pullback in ( 4.6
). However, this would not suffice for the frame
indifference arguments in Section
R is the obvious tensor to pull back the ‘frontleg’ of
( E − G ) .
The physical idea behind the dislocation density tensor α and the inverse elastic distortion W begins by
considering the body in the current configuration and an additive decomposition
of the stress
T = T e
+ T d
, where T e
( t ) is independent of the velocity field at time t .
The fundamental assumption of conventional plasticity [e.g.,
LL67 ] is as follows. Grid the current con
figuration, C , into a union of small, nonintersecting, elements. Now assume that there is a collection of pieces composed of identical , unstressed, elastic material, one corresponding to each element of the grid. These pieces may be of different sizes, but always of same orientation when such orientation can be defined. The collection has the following properties:
1. each piece can be mapped to the corresponding element in the current configuration by a homogeneous deformation. That is, if e x is the element around x ∈ C and p x its corresponding elastic reference ( e x
, p x are sets of points), then there exists an invertible secondorder tensor field F e
( x ) , and a position field f x
, such that f x
( p x
) 7→ e x f x
( X ) = F e
( x ) ( X − X
0
) + x ∀ X ∈ p x
, X
0
∈ p x
;
4
An additive decomposition into equilibrium and viscous parts is partially justified in [ CM64 ].
12
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
2. there exists a function T independent of x , such that
T e
( x ) = T ( F e
( x )) ∀ x ∈ C .
response as described above. In conventional plasticity, the collection { p x
} has a onetoone correspondence with x ∈ C and is called the ‘intermediate configuration’. These definitions naturally extend to timevarying fields with the field F e defined for ( x , t ) and
T e
( x , t ) = T ( F e
( x , t )) , with T independent of time.
Define the inverse elastic distortion tensor
W ( x , t ) := ( F e
( x , t ))
− 1
.
(5.1)
It is often true that curl W = 0 , in which case it is possible that the pieces { p x
: x ∈ C} fit together to form a coherent configuration and, under appropriate topological assumptions, W is the gradient of a position field on C . An example is a deforming elastic material without any dislocations.
By unloading the body, then making small pieces such that there are no incompatibilities remaining in any of the unstressed pieces, and finally rotating all pieces to a common orientation, this procedure provides a route to define the field W from microscopic simulations or experiments.
Thus, we define the departure of W from being a gradient on C as a measure of dislocation density: curl W = − α .
(5.2)
As in the case of the director incompatibility measure, the dislocation density may be physically visualized as an areal density of lines carrying the Burgers vector as a vectorial attribute.
The object W is a twopoint tensor between the current configuration and the intermediate configuration.
The intuition behind the conceptualization of the intermediate configuration implies that for two motions that differ only by a timedependent rigid transformation, the intermediate configuration can be assumed to remain invariant without any loss of physical generality. Thus, under rigid rotations of the current configuration characterized by an orthogonal tensor Q , W transforms as W Q
T
.
We now pose a conservation law for the Burgers vector content of dislocation lines threading any arbitrary area patch in the body, using the same geometric justification as for any welldefined spatial density:
Z a ( t )
˙
αν da = −
Z c ( t )
α × α
V d x
⇒ ˚ = − curl ( α × α
V ) .
(5.3)
Unlike the conservation law for the director incompatibility, there is no geometric source term since the targetspace of W remains invariant under superposed rigid motions of the current configuration. Now,
following similar reasoning as in ( 4.3
not ignoring the vector field gradient that can arise , we have
˙
+ W L = α ×
α
V + grad p .
(5.4)
13
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
In smectic liquid crystals, we associate grad p with the permeation velocity gradient, where permeation refers to the transverse flow of molecules relative to the smectic layers keeping the layers intact
(up to identity of molecules) [ Hel69 ,
Wei97 , Ste07 ]. This is in analogy with crystal plasticity
where such a gradient represents dissipative, compatible permanent deformation that, up to boundary con
unchanged but lattice sites are occupied by different atoms in the course of time. Since the permeation velocity is a field that affects the physics predicted by the model, it requires constitutive specification and may not be thought of in the spirit of a gauge field.
We note that all terms in ( 5.4
) are welldefined in terms of information available from operations on the
current configuration. Of course, the definition of W , α , p depend upon a premultiplying orthogonal tensor (that is constant in time and space) characterizing the orientation of the undistorted reference which is also naturally involved in the definition of the materially uniform response function T . As in material symmetry arguments in standard nonlinear elasticity, the changes induced in W and T cancel each other so that the stress predicted on the current configuration is invariant with respect to the choice of the undistorted reference. In addition, here we also require that if ( W , α , p ) is a set of timedependent
( QW , Qα , Qp )
Q , as indeed they do.
For ease of reference, we collect the field equations of the theory:
ρ ˙ + ρ div v = 0
ρ ˙ = div T + ρ b
ρ n × ¨ = div Λ − X : T + ρ K
Γ ( E − G ) + ( E
˙
G ) + ( E − G ) L = − (curl E ) ×
β
V
˙
+ W L = − (curl W ) × α
V + grad p .
(6.1)
4 , 5 are derived from integral balance laws and hence satisfy jump conditions on sur
faces of discontinuity [ Ach07 ]. On any arbitrary surface with unit normal field
N and moving with normal velocity u
N with respect to the material,
J
− β ×
J
− α ×
β
V − Γ ( E − G )
K
α
V
K
× N =
J
α tan
×
( u
N
N
−
= v
J
·
β tan
N )
( u
K
N
+
− v · N )
K
+
J
αN ⊗ v tan
K
,
J
βN ⊗ v tan
K (6.2) where
J
·
K is the difference of the limiting values of its argument evaluated on either side of the surface of discontinuity, and A tan
:= A − ( AN ) ⊗ N and g tan
:= g − ( g · N ) N are the tangential actions of, respectively, a second order tensor and a vector with respect to an orientation N
nature and includes the situation when the surface is ‘material’ in the sense that its normal velocity (with respect to itself) coincides with that of the material surface it is coincident with instantaneously.
Using the fact that the fields β , α are solenoidal, the local forms of the integral balances for the director incompatibility and dislocation density,
˚
= − curl β × β
V − curl ( Γ ( E − G ))
˚ = − curl ( α × α
V ) ,
(6.3)
14
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal can be expressed in Eulerian form [cf.
∂ β
∂t
∂ α
= − curl ( α × [ v +
α
V ]) ,
∂t
= − curl β × v +
β
V − curl ( Γ ( E − G )) making transparent the relative nature of the dislocation and director incompatibility velocities.
(6.4)
) are capable of geometrically representing loop expansion as demonstrated in Sec
with
α
V inplane with the dislocation loop, being of constant magnitude V and pointwise perpendicular to it. Within this ansatz
, it is interesting to note that the tensorial system ( 6.4
2 reduces to the eikonal equation for front propagation of a scalar field π in two space dimensions and time, ( x, y, t ) , given by
( π t
)
2
= V
2
( π x
)
2
+ ( π y
)
2
.
), we have not included possible solenoidal nucleation terms for the director incompat
ibility and dislocation density fields for simplicity. At this level of generality, they are easily admitted.
the framework and it may even be expected to be the norm in liquid crystalline materials.
In preparation for deducing constitutive guidance on elastic response and dissipative driving forces, we consider a consequence of frameindifference on the free energy density function, ψ , where ψ depends on n , E , W , α , β
. We adapt the presentation of [ ACF99 ] for this purpose. Frame indifference requires
that ψ satisfy
ψ ( n , E , W , α , β ) = ψ Qn , QEQ
T
, W Q
T
, αQ
T
, QβQ
T
(7.1) for all proper orthogonal Q and for all elements n , E , W , α , β in the domain of the function ψ . In
) has to apply for all functions
s → Q ( s ) , 0 ≤ s ∈
R
, with
Q (0) = I ; d Q
(0) = S = − ds d Q
T ds
(0) and S
is an arbitrary fixed skew tensor. Differentiating ( 7.1
s = 0 implies
∂ψ
∂ n
⊗ n +
∂ψ
∂ E
E
T − E
T
∂ψ
∂ E
− W
T
∂ψ
∂ W
− α
T
∂ψ
∂ α
+
∂ψ
∂ β
β
T − β
T
∂ψ
∂ β
: S = 0 and due to the arbitrariness of S we obtain Ericksen’s identity for our model:
∂ψ
∂ n
⊗ n skw
= −
∂ψ
∂ E
E
T − E
T
∂ψ
∂ E skw
+ W
T
∂ψ
∂ W skw
+ α
T
∂ψ
∂ α skw
−
∂ψ
∂ β
β
T − β
T
∂ψ
∂ β skw
(7.2)
.
15
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
In the next section we will use the transformation rule for the partial derivatives of ψ ; we record this rule for only one case below as the rest are similar. Denoting the partial derivative of ψ with respect to its second argument as ∂
E
ψ
∂
E
ψ ( n , E , W , α , β ) = Q
T
∂
E
ψ Qn , QEQ
T
, W Q
T
, αQ
T
, QβQ
T
Q .
(7.3)
We also note that if
X : ( AB ) = d for secondorder tensors A , B and a vector d then
X : QAQ
T
QBQ
T
= Qd , (7.4) which is a direct consequence of the preservation of angles between, and magnitudes of, vectors under the action of an orthogonal tensor.
Assuming a free energy density function ψ with arguments as discussed in Section
the mechanical dissipation D
). We first compute the material time derivative of
ψ :
ψ
˙
=
∂ψ
∂ n
· ˙ +
∂ψ
∂ E
∂ψ
: ˙ +
∂ W
: ˙ +
∂ψ
∂ α
: ˙ +
∂ψ
∂ β
= −
∂ψ
∂ n
+
+
+
+
∂ψ
⊗ n : Γ
∂ψ
: − β ×
β
V − ( E − G ) L + ˙ − Γ ( E − G )
∂ E
∂ψ
∂ α
: ( − α × α
V + grad p − W L )
∂ W
∂ψ
: − div vα + αL
T − curl ( α × α
V )
: − div vβ + βL
T − curl β ×
∂ β
β
V + Γ ( E − G ) .
(8.1)
Some useful formulae for subsequent use are
˙
=
˙ n n − GL ,
A : grad ˙ = ( X : ( n ⊗ A )) : M − AG
T
: Γ = e jki n k
A ip
M jp
− A ip
G kp
Γ ik for an arbitrary secondorder tensor A , and
ρ
∂ψ
∂ β
: curl ( Γ ( E − G )) = − ρ
∂ψ
∂ β
− tr
∂ψ
∂ β
I ( E − G )
T
∂ψ
: M + ρ
∂ β
β
T
: Γ .
Recalling the dissipation ( 3.2
D =
Z
V ( t )
T : L + Λ : M + T : Γ − ρ ψ
˙ dv,
16
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal we collect the terms multiplying L , Γ , M respectively:
Z
V ( t )
T − ρ
"
− E
T
∂ψ
∂ E
− W
T
∂ψ
∂ W
−
Z
Z
V ( t )
V ( t )
T − − ρ
∂ψ
∂ n
∂ψ
⊗ n − ρ
∂ E
E
T
− ρ
∂ψ
∂ β
β
T
∂ψ
Λ − X : n ⊗
∂ E
− ρ
∂ψ
∂ β
− tr
∂ψ
∂ α
∂ψ
∂ β
: α +
∂ψ
∂ β skw
I
:
(
Γ
E
: β I + dv,
− G )
T
∂ψ
∂ α
T
: M dv.
α +
∂ψ
∂ β
T
β
#!
: L dv,
The remaining contributions to the dissipation are:
Z
Z
V ( t )
V ( t ) and
X
X :
:
"
"
ρ
∂ψ
∂ E
+ curl ρ
∂ψ
∂ β
∂ψ
− ρ
∂ W
+ curl ρ
∂ψ
∂ α
T
β
#!
· β
V dv +
Z
∂V ( t )
− ρ
∂ψ
∂ β
: β × β
V × ν da,
T
α
#!
·
α
V dv +
Z
∂V ( t )
− ρ
∂ψ
∂ α
: ([ α ×
α
V ] × ν ) da,
Z
V ( t )
∂ψ
−
∂ W
: grad p dv.
(8.2)
In the spirit of generalizing EL theory, we make the constitutive assumption for the equilibrium part T of the total stress T = T e
+ T d as e
T e
= ρ − E
T
∂ψ
∂ E
− W
T
∂ψ
∂ W
−
∂ψ
∂ α
: α +
∂ψ
∂ β
: β I +
∂ψ
∂ α
T
α +
∂ψ
∂ β
T
β
!
, (8.3) and the couplestress tensor as
∂ψ
Λ = X : n ⊗
∂ E
+ ρ
∂ψ
∂ β
− tr
∂ψ
∂ β
I ( E − G )
T
.
Incorporating these assumptions, the dissipation can now be expressed as
Z
V ( t )
T d sym
: D dv +
Z
V ( t )
T d skw
: Ω − Γ
T
Z
+
V ( t ) dv
T e
+ ρ
∂ψ
∂ n
∂ψ
⊗ n + ρ
∂ E
E
T
+ ρ
∂ψ
∂ β
β
T
+
.
skw
: Γ dv
(8.4)
(8.5)
We first consider the two boundary terms in ( 8.2
). The dependence of the free energy on
α , β accounts for the energy content of individual defect cores, beyond the elastic energy in their stressfields. Mathematically, they act as regularization [cf.
Ach10 , AMZ10 ]. For instance, the dislocation core energy
contribution may look like µb
2
α : α where µ is a shear modulus and b is of the order of the interatomic spacing. Thus, the terms
∂ψ
,
∂ψ are expected to be small away from cores in comparison to typical
∂ β ∂ α derivatives of ψ with respect to E or W . Consequently, constitutive guidelines to ensure nonnegative dissipation in the model will be based only on the bulk terms in the expression for the dissipation.
and subsequent neglect of the boundary term. For the term related to permeation in
we do not follow
17
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal this procedure as it is unclear that the boundary term can be estimated to be small in comparison to the other dissipative contributions.
An essential requirement is that the dissipation in the model be frameindifferent or objective
that the director field transforms as n → Qn under a superposed rigid body motion characterized by the timedependent, spatially uniform orthogonal tensor field Q , it can be seen that T d sym transform objectively, i.e. follow the transformation rule ( · ) 7→ Q ( · ) Q
T
, T d skw
, D , Ω − Γ
T
. Thus, the first two terms in
) transform as objective scalars, i.e. remain invariant under superposed rigid body motions.
By their physical definitions, the director incompatibility and dislocation velocities (with respect to the material), β V , α V , are objective vector fields on the current configuration and therefore have to transform by the rule ( · ) 7→ Q ( · ) under superposed rigid body motions. Due to its twopoint nature, grad p transforms as ( · ) 7→ ( · ) Q
T
. Using the discussion surrounding ( 7.3
transform as objective scalars.
To ensure frameindifferent dissipation, only the third integral in ( 8.5
S ( t ) :=
Q ( t ) Q
T
( t ) , Γ transforms as
Γ 7→ − S + QΓ Q
T under superposed rigid body motions, where arbitrary S generate corresponding funtions Q . Since the coefficient of Γ
) transforms objectively, it has to vanish for the dissipation to transform as an
objective scalar. If not, the dissipation can be made to take arbitrarily different values in motions that differ only by superposed rigidbody motions generated by varying S . To avoid imposing any constraints on the function ψ
beyond those due to frameindifference and material symmetry
coefficient of Γ
) vanish for all admissible choices of
ψ . This is a strong constraint and its satisfac
tion validates the mechanical structure of the theory. Using ( 7.2
A
T
B − B
T
A = 0 skw for any second order tensors A , B , we see that the requirement is indeed satisfied for all frameindifferent
ψ .
We emphasize that the presence of the last two terms in the coefficient of Γ
sequence of the geometric source term in ( 4.2
). Hence, these terms play a crucial role in ensuring the
frameindifference of the theory. Since we are working with a 3d body in 3d Euclidean space the tangent space of a material point is always the same vector space. Consequently, there is no ambiguity in defining material time derivatives of tensor fields unlike in tensor calculus on manifolds. Curiously, however, frameindifference forces the consideration of geometrically ‘proper’ convected derivatives in
ordinary, ‘flatspace’, 3d continuum mechanics as in ( 4.5
Usually, the bulk terms in an expression for dissipation like ( 8.2
) directly indicate the driving forces
for director incompatibility velocity, the dislocation velocity and the permeation velocity gradient as the coefficients of β V , α V , grad p , respectively, in the sense that the absence of these forces render the corresponding dissipative mechanisms nonoperational. Also, the simplest constitutive equations ensuring nonnegative dissipation are constructed by assigning linear relations between members of dissipative
powerconjugate pairs. But here we face an obstacle with the last integral in ( 8.2
the permeation velocity gradient, as it stands, is not necessarily a gradient of a vector field. Moreover, as mentioned above, there is no justification to integrate this term by parts and ignore the resulting boundary contribution.
5 These are notions we use interchangeably with invariance under superposed rigid body motions.
6
T e skw is also expressed in terms of ψ and its derivatives.
18
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
We deal with this by using a StokesHelmholtz decomposition for −
∂ψ
∂ W
=: P stated as
− div grad H
P
H
P
= curl
× n = 0 on ∂V
P ; div H
P
= 0 on V div grad g
P
P = curl H
P
= div P ; (grad g
P
+ grad g
P on V.
− P ) n = 0 on ∂V and
Given a squareintegrable tensor field P with squareintegrable gradients on the body, the decomposition guarantees the existence of a unique tensor field H
P and a unique (up to a constant) vector field g
P
.
Utilizing this decomposition
Z
V ( t )
∂ψ
−
∂ W
: grad p dv =
Z
V ( t ) grad g
P
: grad p dv where the boundary condition on we consider grad g
P
H
P in the StokesHelmholtz decomposition is crucial. Consequently, as the driving force for the permeation velocity gradient
identify driving forces directly from the bulk expressions in ( 8.2
grad p . For
α
V ,
β
V we
In ending this section, we note the decidedly nonlocal nature of the nonnegative dissipation arguments.
Clearly, positive dissipation is guaranteed only in a global sense over the entire body.
The quantities ψ, T , Λ , α V , β V , grad p require constitutive specification. The constitutive choices
T = T e
+ T d
,
T e
= ρ − E
T
∂ψ
∂ E
− W
T
∂ψ
∂ W
−
∂ψ
∂ α
: α +
∂ψ
∂ β
: β I +
∂ψ
∂ α
T d sym
=
identical to restrictions of EricksenLeslie theory [ Les92 ]
,
Λ = X : n ⊗
∂ψ
∂ E
+ ρ
β
V in the direction of X :
"
∂ψ
∂ β
− tr
∂ψ
∂ β
I (
∂ψ
ρ
∂ E
+ curl ρ
∂ψ
∂ β
E −
T
G
β
)
T
#
,
=: f
β
,
α
V in the direction of X :
"
− ρ
∂ψ
∂ W
+ curl ρ
∂ψ
∂ α
T
α
#
=: f
α
,
T
α +
∂ψ
∂ β
T
β
!
,
(9.1) achieve nonnegative dissipation in the model. Reasonable constitutive equations for defect motion may be assumed to be
β
V = m
β f
β f
β
;
α
V = m
α f
α
 f
α

, where m α , m β ≥ 0 are frameindifferent scalar functions. For example, m α =
 f
B
α
α
 with B α a material
 α  constant that characterizes the dislocation drag that arises from energy dissipated at scales that are not resolved by the continuum fields.
19
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
We note that nonnegative dissipation and frameindifference are the only constraints on the kinetic functions for the defect velocity specification.
With regard to a constitutive equation for grad p , any gradient of a vector field on the body satisfies the constraint
Z grad g
P
: grad p dv ≥ 0
V ( t ) and transforms as ( · ) 7→ ( · ) Q
T under superposed rigidbody motions of the current configuration suffices; the notion is not empty as a reasonable and simple choice is
1 grad p =
B P grad g
P
; B
P
> 0 , where B P is a material viscosity constant related to the permeation mechanism.
As examples, we record possible forms of constitutive assumptions for modeling various classes of liquid crystalline materials.
A proposed model is the standard EricksenLeslie nematic liquid augmented with a treatment of director defects. We make the choices
∂ψ
∂ W
∂ψ
≡ 0 ,
∂ α
≡ 0 ,
∂ p
∂ x
≡ 0 ,
α
V ≡ 0 .
5 is simply the kinematic compatibility relationship between the deformation gradient map of the current configuration from any arbitrarily fixed reference configuration and the velocity gradient field on the current configuration. Denoting the deformation gradient from this arbitrary reference as
F := W
− 1
, we note that
˙
= − W L ⇔ F F
− 1
= L .
Thus, this equation is identically satisfied if the current configuration is achieved by a motion of the body that is compatible with the reference at all instant of time.
If the nematic is further assumed to be incompressible, one adds a term − P I
1 incompressibility constraint div v = 0 to account for the and the latter is an additional equation to be solved. Here P is a constitutively undetermined pressure field that is determined by the field equations and boundary conditions.
For the free energy density, one could adopt the OZF form [ Ose33 ,
defect core energy. We make the necessary changes to account for our relaxation of the unit magnitude constraint on n :
˜ := n
; l
1
ψ n
=
2 ρ
0
˜
:=
E
; l k
1
˜
: I
+ ( k
2
+ k
4
)
˜
:=
β l
2
+ k
2
˜ · X E
2
: I − ˜
: I
2
+ k
3
2
˜ ×
+ k
5 l 2
β
˜
X
β
E
2
+ p (  ˜  − 1)
2
.
(9.2)
20
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
Here, k
1
, k
2
, k
3 are the splay, twist, and bend constants; ( k 2 + k
4
) is the saddlesplay constant and k
5 is a modulus related to defect core energies, expected to be of the order of the other standard moduli; l
β is a length of the order of the spatial extent of the cross section of the defect core; and l is the length of the nematic molecule along the director.
E is naturally assumed to be dimensionless (following G ) and the various moduli have the physical units of force or energy per unit length [see e.g.
ρ
0 is the density of the state in which the measurement of the moduli were made and p > 0 is a penalty moduli with units of stress to impose the fixedlength constraint on the director.
We note that while the energy density ( 9.2
) is essentially the same as the OZF energy in the absence of
defects, it deviates from the OZF energy in the presence of defects due to the fact that grad n = E , even when n is locally close to a unit vector field and the core term is ignored. Maintaining the correspondence in the presence of defects appears to be difficult, primarily because of the ambiguity in defining a director field that corresponds to an E in the presence of defects (see Appendices
and
for further discussion).
In correspondence with the elasticity of solids, it is natural to expect that the OZF energy displays nonconvexity in the director distortion at large magnitudes to reflect a breakdown in director elastic strength with increasing director deformation.
A constitutive equation for
β V is required, and a simple form that may be assumed is
β
V = f
β
B β g (  β  )
; g (  β  ) = 1 or  β  where B
β is a defect drag coefficient.
Finally, the viscous stress can follow the EL theory [e.g.
T d
= α
1
( ˜ · D ˜ ) ˜ ⊗ ˜ + α
2
˙˜
− Ω ˜ ⊗ ˜ + α
3
˜ ⊗
˙˜
− Ω ˜ + α
4
D + α
5
( D ˜ ) ⊗ ˜ + α
6
˜ ⊗ D n .
The various α
( · ) are the wellestablished Leslie viscosities.
The model is structurally the same as for the nematic, except for the replacement of k
2 by k
2 t
0
+ ˜ · X E
2
˜ · X E
2
The liquidlike response remains the same as for the nematic. However, there is additionally a solidlike response due to the positional ordering of the smectic layers.
Our model is motivated by those in [ Wei97 , Ste07 ]. We posit an undeformed director
a
0 that characterizes the smectic layer normal in the undistorted elastic reference (Section
 a
0
 being the undistorted interlayer spacing. Now define the deformed layer normal as a = W
T a
0
.
21
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
Then a simple phenomenological energy density for the smectic is
ψ s
= ψ n
+ ψ e
(  a  −  a
0
 ) +
1
2
ρ
0 p s
1 −
 n n
·
  a a 
2
!
+
1
2
ρ
0
µb
2
α : α .
(9.3)
Here, ψ e is a positive scalar function characterizing (positional) elasticity of the smectic layers that penalizes changes in interlayer spacing. The third term penalizes orientations of the layer normal that are not aligned with the director, with p s a penalty modulus with units of stress. In the fourth term, µ is a typical modulus related to the elasticity of layer deformation and b is a length scale of the order of the crosssection of the dislocation core.
A simple constitutive equation for the dislocation velocity
α V that may be assumed is
α
V = f
α
B α g (  α  )
; g (  α  ) = 1 or  α  , where B
α is a dislocation drag coefficient.
The fluid viscous response, i.e. the specification for T d
, is as in nematics. However, a distinguishing
source of nonNewtonian viscosity is slip deformations in the lattice. Extending that analogy to the smectic case, a simple constitutive equation might be grad p = m
P grad g
P where m P permeation.
is a permeation mobility constant that is set to reflect the higher observed viscosity due to
The model is identical to the Smectic A except the third term in ( 9.3
2
!
1
2
ρ
0 p s
1 − n · a
 n   a  changes to
1
2
ρ
0 p s
(cos θ
0
)
2
− n · a
 n   a 
2
!
where θ
0 is the angle between the smecticC layer normal and the director.
We set T d
= 0 in the various liquid crystal models as well as m
P
= 0 for the smectics. We then add an appropriate solid free energy response for the elastomer to obtain a nematic liquid crystal elastomer. A
ψ nc
=
1
2
µ l ( ˜
0
) W
− T l
− 1
( ˜ ) W
− 1
: I , where l is a given symmetric invertible tensorvalued function of ˜ , and ˜
0 field that remains unchanged under superposed rigid body motions.
is a known reference director
22
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
We have relied on four primary design criteria in developing this model:
1. Defects are introduced through geometrically rigorous spatial densities (Euclideanspace analogs of 1,2,3 forms) and the consequent conservation laws.
2. In the absence of defects, the model for liquid crystalline materials should reduce to the Ericksen
Leslie model.
3. The specification of nematic elasticity response must depend only on the current configuration
(both positional and orientational) of the body and not prior states.
4. Defects should be identified as localizations in fields and it should not be necessary to deal with them as individual entities in specifying the rules of dynamic evolution.
Even though very general, and therefore weak, criterion 1 has nonnull content. For example, consider a secondorder tensor order parameter Q which is not known or defined to be a spatial density, i.e., it is not an object that can be integrated along curves, or areas, or volumes. Then, even if one were to write a conservation law for it, the nature of the flux of Q is not clear. For instance, if Q was the volumedensity of a (second order) tensor field (i.e. a second order tensorvalued 3form), the appropriate rate of change of
Q would be the divergence of a third order tensor flux field that represents a second order tensorvalued
2form. On the other hand, if Q were an areal density of a vector field (a vectorvalued 2form), the appropriate time derivative would be the curl of a second order tensor flux field that represents a vectorvalued 1form. Moreover, the appropriate convected time derivatives also take distinctly different forms
. For this reason, despite our high regard for Ericksen’s intuition for the mechanics of
liquid crystals and his seminal contributions to the understanding of these materials, we have reservations about the balance law for the degree of orientation field, S
, in [ Eri91 ]: it is not physically clear to us what
the generalized momentum P (corresponding to S ) represents. A similar comment applies to the corresponding flux, T , although, from the mathematical balance law it is clear that the generalized momentum
P is intended to be a scalarvalued 3form (a volume density of a scalar) and its flux, therefore, is a scalar valued 2form (an areal density of a scalar).
Criterion 1 has practical implications for computation. Conservation forms have advantages for the design of numerical approximation schemes, e.g. based on the finite volume method in computational
fluid dynamics [ LeV02 ], or providing natural weak forms for the finite element method [ LW02 ]. In
combination with Criterion 4, the regularized nature of the auxiliary fields permits us to bypass the
PB03 ]. We emphasize, however, that the kinetic relation between the defect velocity and the
driving force can, in principle, be as complex as necessary to model the material, in marked contrast to
multiscale strategy that can easily incorporate kinetic laws from molecular calculations [e.g. following the procedure outlined in
DJ09 ]. Finally, Criteria 1 and 4 allow a clear separation between the defect
kinetics and the energetics even with the regularization of defects.
7
The (backleg) convected derivative, with respect to a flow, of a 2form ( 2.1
) is naturally different from that of a 1form
a , it equals ˙ + a div v . Essentially, they arise from transport theorems for areas, curves, and volumes, respectively.
23
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
Criterion 2 has important practical consequences as the EL model has been thoroughly validated and there is a wealth of information about these features of the model. There also exists a comprehensive literature on experimental measurements of the material constants [e.g.
Lar99 ]. The practical difficulties
in going to a format farremoved from the EL model can be appreciated from a reading of Sonnet et al.
Criterion 3 is, to us, a physical requirement that can be justified from a molecular basis. In adhering to
this, our model stands at odds with that presented in [ ACF99 ].
With respect to Smectic A response, our elastic response function for the couple stress tensor differs
discussed in Section
). The flow viscosity coefficients admitted in [ Ste07 ] are more
general than in EL theory and consequently ours. Stewart’s smectic A model is a mechanically sound
generalization of E’s model [ Wei97 ], making clear the manner in which balance of angular momentum
and the couple stress tensor are to be understood in the latter theory. A fundamental construct of both models is a field equation for the ‘layer variable’ whose evolution uses a newlyintroduced ‘permeation
Smectic A response represents a gradual transition of the liquid crystalline material towards positional order characteristic of solids and defects in such ordering, and we believe that the ‘extranematic’ response is best posed in the context of positional kinematics and elasticity of solids.
strates a practical theory for liquid crystal polymers that is capable of predicting the occurrence of discli
procedure with several closure assumptions provides an evolution equation for the second moment of the distribution function in Doi’s theory. An asymmetric stress tensor for a nonsimple material is intro
duced, following Feng et al. [ FSL00
], and a result from Doi and Edwards [ DE88 ] is used to justify a
‘body torque’ that balances the torque produced by the skew symmetric part of the stress. A similar
model is utilized to understand defect morphology and dynamics in Yang et al. [ YFMW09 ]. The fun
damental basis of our model is obviously very different from these approaches, especially the treatment of angular momentum balance and the operational dissipative mechanisms. However, our model shares features with these works in being able to deal with defects, seamless interpolation between the solid and liquidlike states, and the relative ease (expected, in our case) of practical computation. Hence, it would be useful to compare future predictions that emerge from a numerical implementation of our model.
Criteria 1 and 4 enable computation of defects by recognizing that incompatibilities in the director distortion field are associated with multivalued director field when defects are present. Therefore, our approach utilizes welldefined defect density fields instead of a multivalued director field. This feature has significant implications for the practically important task of defect detection through a local tool, as
of a director field away from defect cores, e.g. as preprocessing to provide initial conditions to our model, or as postprocessing to calculate derived otpical properties. Hence, in Appendix
we provide a pragmatic algorithm to reconstruct a director field that is consistent with given defect fields. We emphasize, however, that our theory does not require such a definition. A related issue is the construction of defect fields in our theory when the disclination is specified in terms of classical quantities such as disclination strength. In Appendix
B , we provide some details on this question. We also explain there
how our theory allows for defects that include disclinations, but are more general.
24
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
We believe that this work is the first to lay out a geometrically exact framework for the study of both orientational and positional defects in liquid crystal materials. This can enable the study of a rich class of theoretical questions and physical phenomena in liquid crystalline materials spanning the liquid to
W ) in a liquid crystal elastomer can become incompatible in the presence of a radial hedgehog defect in the nematic director field. In conventional liquid crystal elastomer models, this is a serious practical problem as an incompatible total deformation requires abandoning the fundamental kinematics; this leads
Fried and Sellers to question the validity of the assumed defect structure or the constitutive equations in their static calculations. In our setting, this merely describes a dislocation defect in the positional order associated with a hedgehog defect in the orientational order, and what persists in time is decided by dynamics that is, at the least, approximately computable. As is known, disclinations in bulk are observed
mechanism of timedependent deformation for polymers is nonlinear viscoelasticity, and this can be
modeled within our framework by a straightforward augmentation following the ideas of [ Doi81 ] and
It is a pleasure to acknowledge discussions with Shelley Anna, Kaushik Bhattacharya, Chuck Gartland and Mark Warner. Support from the US ONR, Grant No. N000140910301 (AA) is gratefully acknowledged. The work of Kaushik Dayal was supported by AFOSR (FA95500910393).
Recall that the director incompatibility field is expressed as curl( E − G ) = β .
We note that at spatial locations where β = 0 , E can differ from G by the value of the gradient of a
locally defined vector field (this is allowed by ( 4.5
)). This is important because localized defects have
nonvanishing, irrotational elastic director distortion fields in domains excluding the defect cores. Thus, even away from defect cores, E and G are not pointwise coincident:
E =: grad ˆ = grad n away from defect cores , (A.1) where the first equality requires interpretation. When E is incompatible on the body, i.e. there is a region where β is nonvanishing, it is not possible to uniquely define a field ˆ even up to a constant vector field. We emphasize that our theory does not require such a definition. However, the classical theory, e.g.
SS74 , Ste04 ], implicitly requires such a construct. We consider that contrast and related issues
in this section.
The interest in liquid crystalline materials is driven in large part by their unusual optical properties. The director field away from defect cores is the primary contributor to these properties. Hence, we outline methods to construct the director field in regions away from the defect cores. While the pair n ,
ˆ that emerges from the Helmholtz decomposition mentioned in the Introduction would seem to contain this
25
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
, we leave a careful characterization of this information content for future work. Instead,
we outline possible pragmatic algorithms to reconstruct a director field, e.g. to use in calculating optical properties. As stated in the Introduction, we shall require that the field n , whether given or constructed, satisfies the unit magnitude constraint at least approximately; however, the field ˆ need not.
The problem with defining a continuous ˆ field may be understood as follows: if the gradient field of a continuous function was to exist, with the gradient matching the smooth E field outside the core region, then the line integral of the gradient on any closed curve surrounding the core would vanish. But the line integral of E along such a closed curve surrounding the core cannot vanish. Thus, such a continuous function cannot exist.
A pointwise spatial gradient, say based on finite differences, of the observed director field can be calculated. This spatial gradient can then be smoothed and set equal to E and the defect field is derived from
β := curl E . We emphasize that smoothing does not necessarily make E compatible, especially if the observed field contains defects. A StokesHelmholtz projection can then be performed via
1 Z min r
2
V
(grad r − E ) : (grad r − E ) + p
 r l

− 1
2
!
dv p 1 , where l is the nematic molecular length along the director direction and p is a nondimensional penalty parameter. A minimizer over all smooth unconstrained vector fields on the body yields an n field that may be required as input to the theory, e.g. as initial condition.
The field E is irrotational away from cores. Therefore a formal vector ‘field’ ˆ can be constructed such that E = grad ˆ
away from cores, e.g. adapting the formula of Bârz˘a [ Bâr05 ], see next subsection. As
constructed the field ˆ may not be a unit vector field; a possible prescription for an approximate unit vector field is to take the corresponding unit norm field.
Continuously differentiable irrotational (curlfree) vector fields on nonsimply connected domains are not necessarily gradients of scalar fields. The following result provides an explicit formula for the ‘non
gradient’ part of such an irrotational vector field. The result is due to Bârz˘a [ Bâr05 ].
Let C
1
, C
2
, . . . C n be n pairwise disjoint curves (i.e., C i
∩ C j
= ∅ for every i = j ), each diffeomorphic to either a straight line or a circle. Further, let C i by f i 1
, f i 2
:
R
3 →
R where f i 1
, f i 2 be generated as the intersection of two surfaces defined are differentiable as many time as required. For each i , at any
( x, y, z ) ∈
R
3 where f 2 i 1
+ f 2 i 2
> 0 , let the gradients of f i 1 and f i 2 not vanish. Define the zeroset surfaces of f i 1 and f i 2 as
S ik
= ( x, y, z ) ∈
R
3  f ik
( x, y, z ) = 0 , k = 1 , 2; i = 1 to n
8
Indeed, even more information: the state of average molecular orientation within defect cores.
26
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal and let C i
= S i 1
∩ S i 2
. Define scalar fields G ik
:
R
3 \ S ik
→
R
, i = 1 to n ; k = 1 , 2 as
G i 1
( x, y, z ) := arctan f
2
( x, y, z ) f
1
( x, y, z )
; G i 2
( x, y, z ) := − arctan f
1
( x, y, z ) f
2
( x, y, z )
Define the vector fields E i
:
R
3 \ C i
→
R
3 as:
1
E i
:= f 2 i 1
+ f 2 i 2 f i 1
∂f
∂x i 2
− f i 2
∂f i 1
∂x
, f i 1
∂f i 2
∂y
− f i 2
∂f i 1
∂y
, f i 1
∂f i 2
∂z
− f i 2
∂f i 1
∂z and note that grad G ik
= E i on R
3 \ S ik
, i = 1 to n, k = 1 , 2
Let the domain Ω :=
R
3 \ ∪ n i =1 can be verified that
C i
. For each i , let γ i
I be any small circle with center at a point of
E i
· d x = ± 2 π
C i
. It
γ i so that E i is not a gradient of a gradient in Ω .
C 1 scalar field in Ω . Note that grad G ik
, i = 1 to n ; k = 1 , 2 is not a
Theorem (Bârz˘a): For E : Ω →
R
3 such that the vector field F : Ω →
R
3 an irrotational vector field in Ω , there exist constants α i
, i = 1 to n defined by
F := E − n
X
α i
E i i =1 is the gradient of a C 1 scalar field on Ω . The constants α i are defined by
α i
=
H
E · d x
γ i
H
γ i
E i
· d x
Thus, for some purposes F + n
X
α i
E i may be formally considered a gradient of a discontinuous scalar i =1 field in Ω .
The nonuniqueness in the definition of an ˆ field referred to in the beginning of this appendix arises from the possibility of more than one distinct set of two surfaces S ik
, k = 1 , 2 , i fixed, defining the same defect curve C i
.
The director defects that are admissible in our model include disclinations but are more general. This is because we have been unable to fit a coordinateindependent definition of disclinations into a generaliza
order parameter field could be introduced with its spatial incompatibilities related to disclinations, but giving this construct a physical interpretation within a singledirector theory like EL is difficult, if not
to introduce new order parameters into the energy at will; in contrast, in our model there is not much room to introduce an additional orientational orderparameter field in the free energy density once we have commited to a director field and balance of linear and angular momentum along with directorbased orientational elasticity.
27
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
Unit vectors are parametrized (at least locally) by two parameters. Consider any such parametrization
( θ
α
: α = 1 , 2) . Specifically, we think of the θ
α as parametrizations of the unit sphere by angles from some fixed orthonormal frame, Figure
3 . Denote a generic point on the sphere by the unit vector
cos θ
2 cos θ
1 e x
+ cos θ
2 sin θ
1 e y
+ sin θ
2 e z where e x
, e y
, e z are the unit vectors along the axes of the frame.
Figure 3: Director incompatibility defect lines.
Now for fixed α , consider the vector field of disclination density d
α i
= ∆θ
α l i
, (B.1) where ∆θ α is a specified constant in radians and l is a specified vector field (the line direction) with compact support on a small cylinder along the disclination curve.
l has physical dimensions of reciprocal area. For brevity, we consider the straight disclination. Then, the vector field l may be defined as l = A ( x ) t , where t is a constant unit vector in the line direction of the disclination and A is any smooth scalar function supported on the core cylinder such that the integral of A over the core crosssection is unity. If we try to generate a function θ
α from the equation curl grad θ
α
= d
α
, we observe that the only possibility of a solution is if it is multivalued, and further that along closed circuits enclosing the core the value of θ α changes by exactly ∆θ α . We note that this exercise is simply to aid intuition and we do not use multivalued fields in our work.
Having chosen an orthonormal frame to define the spherical angles, we adopt the procedure above to define disclinations. It is similar to the classical theory up to the smoothing of the cores. Unfortunately,
28
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal this definition is not independent of the frame. While it is suited to specifying the topological charge of a disclination field containing many disclination loops, it is currently not clear to us how to define the disclination density field in a coordinateinvariant manner and fit such a construct into a generalized
EricksenLeslie theory.
Of course, regardless of our difficulties above, disclinations are observed discontinuities in the director field. Appendix
outlined practical strategies to make approximate connections.
Given solenoidal disclination fields d
α
, we solve for vector fields Θ
α from the equations curl Θ
α
= d
α
, div Θ
α
= 0 .
(B.2)
This is a standard problem of potential theory. The Θ
α are irrotational outside the core region. The result
in [ Bâr05 ] provides a construction to formally express
Θ
α as gradients of scalar fields θ
∗ α
, i.e.
grad θ
∗ α
= Θ
α
(B.3) in the punctured domain consisting of the body without the core cylinders, see Appendix
θ
∗ α are generally not defined on specific surfaces of the body. These scalar spherical angle ‘functions’ immediately define a field, say n
∗
, away from defect cores and the ‘singular’ surfaces.
Away from the cores, an alternative way of generating E for a given disclination configuration is to simply calculate grad n
∗ wherever it is welldefined.
A natural question to ask is how a given disclination density such as d
α may be described directly in terms of the field variables of the theory, in particular E , β . Partial progress towards the answer can be made by considering the composition of an arbitrarily smooth function, say f , with a smooth vector field, say n , on the body, the latter being welldefined at each point of the body. Then f
,j
=
∂f
∂n i n i,j
⇒ 0 = e rkj f
,jk
= e rjk
∂f
∂n i n i,j
,k
= e rkj
∂ 2 f
∂n i
∂n p n p,k n i,j
+
∂f
∂n i n i,jk
.
Motivated by the above formula, it seems that the system of equations curl E = β d
α
= X E
T
A
α
E + β
T a
α
, α = 1 , 2
(B.4) is relevant to the specification of disclination defect fields on the body in terms of E , β , where A
α
, a α d
α and are respectively a symmetric tensorvalued field and two vectorvalued fields that may be specified.
29
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
With reference to Figure
∆θ 1 = 2 πm where m is the strength of the disclination and l is in the direction of z for a wedge disclination, and in the directions x or y for the twist disclination.
Define d
∗ 1 from these ingredients. Equilibrium for the 1constant director elastic energy is characterized
div grad θ
1
= 0 .
(B.5)
d
∗ 1
2
. Thus, the field n
∗ as data be defined from θ
∗ 2
θ
∗ 1
≡
. Then, grad θ
∗ 1
0 , θ
∗ 1
gives an equilibrium director field away from the cores (and singular surfaces) corresponding to the disclinations involved, and this may also be considered as the ˆ field (Appendix
In more complicated cases where equilibrium is not characterized by ( B.5
) away from cores, e.g. if the
α
1constant energy is not invoked, the only change in the argument is to add a gradient, say grad θ , to
1
(which keeps the topological charge of the solution intact) and determine this extra field θ
α as a solution to the more involved equilibrium equation where the θ
∗ α act as forcing fields. The overall director field, ˆ , away from cores arises from the parameters θ
α
+ θ
∗ α : α = 1 , 2 .
[ACF99] D.R. Anderson, D.E. Carlson, and E. Fried, A continuummechanical theory for nematic elastomers , Journal of Elasticity 56 (1999), no. 1, 33–58.
[Ach03] A. Acharya, Driving forces and boundary conditions in continuum dislocation mechanics , Proceedings of the Royal Society of London. Series A: Mathematical, Physical and
Engineering Sciences 459 (2003), no. 2034, 1343.
[Ach04] , Constitutive analysis of finite deformation field dislocation mechanics , Journal of the Mechanics and Physics of Solids 52 (2004), no. 2, 301–316.
[Ach07] , Jump condition for GND evolution as a constraint on slip transmission at grain boundaries , Philosophical magazine 87 (2007), no. 8, 1349–1359.
[Ach10] , New inroads in an old subject: Plasticity, from around the atomic to the macroscopic scale , Journal of the Mechanics and Physics of Solids 58 (2010), 766–778.
[AK91a] R. Abeyaratne and J.K. Knowles, Implications of viscosity and straingradient effects for the kinetics of propagating phase boundaries in solids , SIAM Journal on Applied Mathematics 51 (1991), no. 5, 1205–1221.
[AK91b] , Kinetic relations and the propagation of phase boundaries in solids , Archive for rational mechanics and analysis 114 (1991), no. 2, 119–154.
[AMZ10] A. Acharya, K. Matthies, and J. Zimmer, Wave solutions for a quasilinear model of Field
Dislocation Mechanics , submitted.
[Bâr05] I. Bârz˘a, On the Structure of Some Irrotational Vector Fields , General Mathematics 13
(2005), 9–20.
30
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
[BB98] JS Bergstr
"om and MC Boyce, Constitutive modeling of the large strain timedependent behavior of elastomers , Journal of the Mechanics and Physics of Solids 46 (1998), no. 5, 931–954.
[BM09] JM Ball and A. Majumdar, Nematic liquid crystals: from MaierSaupe to a continuum theory , Oxford University Eprints archive (2009).
[BWT94] P. Bladon, M. Warner, and EM Terentjev, Orientational order in strained nematic networks ,
Macromolecules 27 (1994), no. 24, 7067–7075.
[BZ08] J.M. Ball and A. Zarnescu, Orientable and nonorientable line field models for uniaxial nematic liquid crystals , Molecular Crystals and Liquid Crystals 495 (2008), no. 1, 221–
233.
[CF06] Y. Chen and E. Fried, Uniaxial nematic elastomers: constitutive framework and a simple application , Proceedings of the Royal Society A: Mathematical, Physical and Engineering
Science 462 (2006), no. 2068, 1295.
[CG67] BD Coleman and M. Gurtin, Thermodynamics with internal variables , J. Chem. Phys 47
(1967), no. 2, 85–98.
[CLV01] M.C. Calderer, C. Liu, and K. Voss, Smectic A liquid crystal configurations with interface defects , Mathematical Methods in the Applied Sciences 24 (2001), no. 7, 473–489.
[CM64] B.D. Coleman and V.J. Mizel, Existence of caloric equations of state in thermodynamics ,
The Journal of Chemical Physics 40 (1964), 1116.
[CN63] B.D. Coleman and W. Noll, The thermodynamics of elastic materials with heat conduction and viscosity , Archive for Rational Mechanics and Analysis 13 (1963), no. 1, 167–178.
[DB06] K. Dayal and K. Bhattacharya, Kinetics of phase transformations in the peridynamic formulation of continuum mechanics , Journal of the Mechanics and Physics of Solids 54 (2006), no. 9, 1811–1842.
[DE88] M. Doi and SF Edwards, The theory of polymer dynamics , Oxford University Press, USA,
1988.
[DGJ98] T.A. Davis and E.C. Gartland Jr, Finite element analysis of the Landaude Gennes minimization problem for liquid crystals , SIAM Journal on Numerical Analysis 35 (1998), no. 1, 336–362.
[dGP95] P.G. de Gennes and J. Prost, The physics of liquid crystals , Oxford University Press, USA,
1995.
[DJ09] K. Dayal and R.D. James, Nonequilibrium molecular dynamics for bulk materials and nanostructures , Journal of the Mechanics and Physics of Solids (2009).
[Doi81] M. Doi, Molecular dynamics and rheological properties of concentrated solutions of rodlike polymers in isotropic and liquid crystalline phases , Journal of Polymer Science: Polymer Physics Edition 19 (1981), 229–243.
31
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
[DP91] C. Davini and G.P. Parry, A complete list of invariants for defective crystals , Proceedings:
Mathematical and Physical Sciences 432 (1991), no. 1886, 341–365.
[DV80] IE Dzyaloshinskii and GE Volovick, Poisson brackets in condensed matter physics , Annals of Physics 125 (1980), no. 1, 67–97.
[DWH06] A.M. Donald, AH Windle, and S. Hanna, Liquid crystalline polymers , Cambridge Univ Pr,
2006.
[Eri61] JL Ericksen, Conservation laws for liquid crystals , Journal of rheology 5 (1961), 23.
[Eri91] , Liquid crystals with variable degree of orientation , Archive for Rational Mechanics and Analysis 113 (1991), no. 2, 97–120.
[Fle77] W.H. Fleming, Functions of several variables , Springer, 1977.
[Fra58] FC Frank, I. Liquid crystals. On the theory of liquid crystals , Discussions of the Faraday
Society 25 (1958), 19–28.
[FS06] E. Fried and S. Sellers, Incompatible strains associated with defects in nematic elastomers ,
The Journal of chemical physics 124 (2006), 024908.
[FSL00] JJ Feng, G. Sgalari, and LG Leal, A theory for flowing nematic polymers with orientational distortion , Journal of Rheology 44 (2000), 1085.
[GHL
+
10] EC Gartland, H. Huang, OD Lavrentovich, P. PalffyMuhoray, II Smalyukh, T. Kosa, and
B. Taheri, ElectricField Induced Transitions in a Cholesteric LiquidCrystal Film with
Negative Dielectric Anisotropy , Journal of Computational and Theoretical Nanoscience 7
(2010), no. 4, 709–725.
[GM84] DJ Graziano and MR Mackley, Shear induced optical textures and their relaxation behaviour in thermotropic liquid crystalline polymers , Molecular Crystals and Liquid Crystals 106 (1984), no. 1, 73–93.
[Hal72] I. Haller, Elastic Constants of the Nematic Liquid Crystalline Phase of p
MethoxybenzylidenepnButylaniline (MBBA) , The Journal of Chemical Physics 57
(1972), 1400.
[Hel69] W. Helfrich, Capillary flow of cholesteric and smectic liquid crystals , Physical Review
Letters 23 (1969), no. 7, 372–374.
[Hil78] R. Hill, Aspects of invariance in solid mechanics , Advances in applied mechanics 18
(1978), 1–75.
[KF08] M. Kleman and J. Friedel, Disclinations, dislocations, and continuous defects: A reappraisal , Reviews of Modern Physics 80 (2008), no. 1, 61–115.
[Kin91] D. Kinderlehrer, Recent developments in liquid crystal theory , Frontiers in pure and applied mathematics: a collection of papers dedicated to JacquesLouis Lions on the occasion of his sixtieth birthday, ed. R. Dautray, Elsevier, New York (1991), 151–178.
32
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
[KLGCC08] D.H. Klein, L.G. Leal, C.J. GarcíaCervera, and H.D. Ceniceros, Threedimensional sheardriven dynamics of polydomain textures and disclination loops in liquid crystalline polymers , Journal of Rheology 52 (2008), 837.
[Lar99] RG Larson, The structure and rheology of complex fluids , Oxford University Press, 1999.
[Les68] FM Leslie, Some constitutive equations for liquid crystals , Archive for Rational Mechanics and Analysis 28 (1968), no. 4, 265–283.
[Les92] , Continuum theory for nematic liquid crystals , Continuum Mechanics and Thermodynamics 4 (1992), no. 3, 167–175.
[LeV02] R.J. LeVeque, Finite volume methods for hyperbolic problems , Cambridge Univ Pr, 2002.
[LL67] EH Lee and DT Liu, FiniteStrain Elasticâ ˘ TPlastic Theory with Application to Plane
Wave Analysis , Journal of Applied Physics 38 (1967), no. 1, 19–27.
[LL00] F.H. Lin and C. Liu, Existence of solutions for the EricksenLeslie system , Archive for
Rational Mechanics and Analysis 154 (2000), no. 2, 135–156.
[LP94] F.H. Lin and C.C. Poon, On Ericksen’s model for liquid crystals , Journal of Geometric
Analysis 4 (1994), no. 3, 379–392.
[LW00] C. Liu and N.J. Walkington, Approximation of liquid crystal flows , SIAM Journal on Numerical Analysis 37 (2000), no. 3, 725–741.
[LW02] , Mixed methods for the approximation of liquid crystal flows , Mathematical Modelling and Numerical Analysis 36 (2002), no. 2, 205–222.
[MZ09] A. Majumdar and A. Zarnescu, Landau–De Gennes Theory of Nematic Liquid Crystals: the Oseen–Frank Limit and Beyond , Archive for Rational Mechanics and Analysis (2009),
1–54.
[Nol67] W. Noll, Materially uniform simple bodies with inhomogeneities , Archive for Rational Mechanics and Analysis 27 (1967), no. 1, 1–32.
[Ose33] CW Oseen, The theory of liquid crystals , Transactions of the Faraday Society 29 (1933), no. 140, 883–899.
[PB03] P.K. Purohit and K. Bhattacharya, Dynamics of strings made of phasetransforming materials , Journal of the Mechanics and Physics of Solids 51 (2003), no. 3, 393–424.
[Pei40] R. Peierls, The size of a dislocation , Proceedings of the Physical Society 52 (1940), no. 1,
34–37.
[Pra57] S. Prager, Stressstrain relations in a suspension of dumbbells , Journal of Rheology 1
(1957), 53.
[SKH95] A. Sonnet, A. Kilian, and S. Hess, Alignment tensor versus director: Description of defects in nematic liquid crystals , Physical Review E 52 (1995), no. 1, 718–722.
33
Continuum Mechanics of Line Defects in Liquid Crystals and Liquid Crystal Elastomers A. Acharya and K. Dayal
[SMV04] AM Sonnet, PL Maffettone, and EG Virga, Continuum theory for nematic liquid crystals with tensorial order , Journal of NonNewtonian Fluid Mechanics 119 (2004), no. 13, 51–
59.
[SS74] M.J. Stephen and J.P. Straley, Physics of liquid crystals , Reviews of Modern Physics 46
(1974), no. 4, 617–704.
[SSF09] O.E. Shklyaev, A.Q. Shen, and E. Fried, Evolution equation for a disclination line located between the uniaxial and isotropic phases of a nematic liquid crystal , Journal of colloid and interface science 329 (2009), no. 1, 140–152.
[Ste04] I.W. Stewart, The static and dynamic continuum theory of liquid crystals: a mathematical introduction , CRC, 2004.
[Ste07] , Dynamic theory for smectic A liquid crystals , Continuum Mechanics and Thermodynamics 18 (2007), no. 6, 343–360.
[SZA06] S.A.S.L. ShojaeiZadeh and S.L. Anna, Role of surface anchoring and geometric confinement on focal conic textures in smecticA liquid crystals , Langmuir 22 (2006), no. 24,
9986–9993.
[Tar10] L. Tartar, The general theory of homogenization: a personalized introduction , Springer
Verlag, 2010.
[Wei97] E. Weinan, Nonlinear Continuum Theory of SmecticA Liquid Crystals , Archive for Rational Mechanics and Analysis 137 (1997), no. 2, 159–175.
[WT07] M. Warner and E.M. Terentjev, Liquid crystal elastomers , Oxford University Press, USA,
2007.
[YFMW09] X. Yang, M.G. Forest, W. Mullins, and Q. Wang, Dynamic defect morphology and hydrodynamics of sheared nematic polymers in two space dimensions , Journal of Rheology 53
(2009), 589.
[Zoc33] H. Zocher, The effect of a magnetic field on the nematic state , Transactions of the Faraday
Society 29 (1933), no. 140, 945–957.
34